# Nanofluid optical property characterization: towards efficient direct absorption solar collectors

- Robert A Taylor
^{1}Email author, - Patrick E Phelan
^{1}, - Todd P Otanicar
^{2}, - Ronald Adrian
^{1}and - Ravi Prasher
^{1}

**6**:225

https://doi.org/10.1186/1556-276X-6-225

© Taylor et al; licensee Springer. 2011

**Received: **31 October 2010

**Accepted: **15 March 2011

**Published: **15 March 2011

## Abstract

Suspensions of nanoparticles (i.e., particles with diameters < 100 nm) in liquids, termed nanofluids, show remarkable thermal and optical property changes from the base liquid at low particle loadings. Recent studies also indicate that selected nanofluids may improve the efficiency of direct absorption solar thermal collectors. To determine the effectiveness of nanofluids in solar applications, their ability to convert light energy to thermal energy must be known. That is, their absorption of the solar spectrum must be established. Accordingly, this study compares model predictions to spectroscopic measurements of extinction coefficients over wavelengths that are important for solar energy (0.25 to 2.5 μm). A simple addition of the base fluid and nanoparticle extinction coefficients is applied as an approximation of the effective nanofluid extinction coefficient. Comparisons with measured extinction coefficients reveal that the approximation works well with water-based nanofluids containing graphite nanoparticles but less well with metallic nanoparticles and/or oil-based fluids. For the materials used in this study, over 95% of incoming sunlight can be absorbed (in a nanofluid thickness ≥10 cm) with extremely low nanoparticle volume fractions - less than 1 × 10^{-5}, or 10 parts per million. Thus, nanofluids could be used to absorb sunlight with a negligible amount of viscosity and/or density (read: pumping power) increase.

## Introduction

Nanofluids, or suspensions of nanoparticles in liquids, have been studied for at least 15 years and have shown promise to enhance a wide range of liquid properties [1–20]. In the last few years, the co-authors [21–23] and others [24, 25] have explored their potential towards developing a new type of direct absorption (or volumetric) solar thermal collector. The ideal volumetric thermal collector should: (1) efficiently absorb solar radiation (in the wavelength range - 0.25 < *λ* < 2.5 μm) and convert it to heat directly inside the working fluid, (2) minimize heat losses by convection and radiation (in the wavelength range - *λ* > 4 μm), and (3) keep system fouling/clogging and pumping costs to a minimum. The focus of this article is to explore condition (1) in detail for nanofluids.

where *μ*_{eff} and *μ*_{f} refer to the effective nanofluid viscosity and the base fluid viscosity, respectively. Also, *C*_{μ} can be found through a relation to several other fluid parameters - see [28]. For many cases, though, *C*_{μ} = 10 is a reasonable approximation [28]. If we plug in *f*_{v} < 1 × 10^{-5}, we can see that there is a negligible change in viscosity (i.e., *μ*_{eff} ≈ *μ*_{f}). If viscosity is unchanged, it is even less likely that density would change at these low volume fractions. Thus, pumping power (for a *stable* nanofluid) will not change. For these reasons, nanofluids compare favorably with black dye and micro/macroparticle laden liquids. They are also expected to show enhancement over conventional surface-based collectors [21–25].

On the other hand, recent research indicates that nanofluids must be very carefully chosen to match their application in order to see enhancement. This is especially true for the nanofluid optical properties in a solar collector. If the volume fraction of nanoparticles is very high, all the incoming light will be absorbed in a thin surface layer where the thermal energy is easily lost to the environment. On the other hand, if the volume fraction of nanoparticles is low, the nanofluid will not absorb all the incoming solar radiation. Therefore, the optical properties of the fluid must be controlled very precisely or a nanofluid could actually be detrimental in a solar collector. This article first describes some simple modeling (using bulk properties) approaches that we used to explore how a nanofluid absorb sunlight. Next, we will describe our experimentation methods towards this same end. These results will then be compared and discussed. Lastly, this study presents some nanofluid recipes with cost estimates for solar collector applications.

## Modeling approach

*α*, in Figure 1 is defined as [30]:

*D*is the diameter of the nanoparticle and

*λ*is the wavelength of incident light (note:

*D*and

*λ*must be of the same units to get a non-dimensional

*α*). Thus, very small particle sizes and volume fractions make it is safe to assume that we are working in the independent scattering regime which requires relatively simplistic optical properties calculations. Commonly used nanoparticles are in the range 10 to 50 nm of average particle diameter, for which most of the incident light from the sun has a wavelength that is at least ten times larger. This allows one to ignore many of the higher order components found in Mie scattering theory [31]. As a result, the following equations can be used to solve for the scattering (

*Q*

_{scat}), absorption (

*Q*

_{abs}), and extinction (

*Q*

_{ext}) efficiencies, respectively, of individual particles. (These equations are found in several standard texts, such as Bohren and Huffman [32].)

where *m* is the relative complex refractive index of the nanofluid and *α* is the size parameter, which depends on the particle diameter, *D*, and the incident wavelength, *λ* [31].

*Q*

_{scat}is generally at least an order of magnitude smaller than

*Q*

_{abs}due to the fact that scattering is proportional to

*D*

^{4}. Consequently, scattering is usually negligibly small. However, this is only true if the particles are uniformly small. In reality, some fraction of the fluid may consist of larger particle agglomerates. If it is negligible, the scattering coefficient simply drops out of the following equation for the nanoparticles' extinction coefficient,

*σ*

_{particles}[32]:

*σ*

_{basefluid}, and that of the particles,

*σ*

_{particles}. We define these as the following:

*k*

_{basefluid}is the complex component of the refractive index for the base fluid. Also, for comparison with other research, we choose to present extinction coefficients in cm

^{-1}. This means that

*λ*and the fluid depth,

*L*, must be in cm in the following equation of Beer's law [32]:

### Effective medium approach to optical properties

*ε*

_{f}is very small, as it is in the complex dielectric component for water (from 0.1 to 1 μm), large rounding errors may occur when using this approach. This limits the applicability of this method. Once the effective dielectric constant is found, it is relatively easy to convert back to the refractive index using [32]:

*ε*' and

*ε*" represent the real and imaginary components of the dielectric constant. The real part,

*n*

_{eff}, of the refractive index for several nanofluids, determined from Equations 11 and 12, is plotted in Figure 2. Since there is, at most, a factor of ten difference (and in many cases less than 100% change) in the real part of the refractive index between the bulk particle material and the base fluid, this approach gives rather accurate results. Figure 2 shows little deviation from the real part of the refractive index for low volume fractions, which is logical. Note: Properties for the bulk materials were taken from Palik [29] for the effective medium analysis.

*k*

_{eff}, the effective medium approach yields a severe underprediction. For the sake of consistency, Figure 3 also plots extinction coefficients, which are calculated using Equation 7, with

*k*

_{eff}replacing

*k*

_{basefluid}. The results given in Figure 3 are many orders of magnitude below the measured values for these volume fractions. In the visible range,

*k*

_{eff}for water is many orders of magnitude (approximately ten) less than that of metal nanoparticles. Due to this large difference, the Maxwell-Garnett theory is generally not an accurate approach to obtain the extinction coefficient for nanofluids.

### Scattering issues

where *D* is the particle diameter, *N* the number of scattering particles in the beam path, *λ* the wavelength of light, *m* the relative complex refractive index, and *θ* the scattering angle. Thus, a tripling of the diameter (from 30 to 90 nm) gives a 730-fold increase in the amount of scattering! Thus, if particles in a real nanofluid are larger than what is assumed above, scattering may cause deviations from the model.

## Experimental approach

Creating a stable nanofluid is a must for any real application and for measuring optical properties. Without careful preparation, nanoparticles will agglomerate and settle out of the base fluid in a very short time. Although there are many methods of nanofluid preparation, they can be roughly categorized into "one-step" and "two-step" processes. One-step processes synthesize the nanofluid to the desired volume fraction and particle size inside the base fluid. Thus, the final product is a specific nanofluid which is ready for use (possibly after dilution). The two-step method is accomplished by first synthesizing the dry nanoparticles to a preferred size and shape. In the second step, these particles are carefully mixed into the desired base fluid at the desired volume fraction, usually with some additives for stability.

Several researchers have had success fabricating and testing nanofluids using one-step preparation methods [33–35]. Based on these results, one-step methods may produce the best results for commercial applications if they can be scaled up and manufactured inexpensively. However, due to its straightforward nature and its controllability, we will only use and discuss the two-step method.

A variety of dry powders are available "off-the-shelf" [36–38]. These particles can be mixed into many different liquids at the preferred concentration. Depending on the stability and quality required, this process can take anywhere from a few minutes to several hours. For the test fluids of this article, the particles and up to 1% sodium dodecyl sulfate (a surfactant) were dispersed into the base fluid using a sonicator (a UP200 from Hielscher Ultrasonics GmbH, Teltow, Germany) for 15 to 30 min. From our experience, probe-type sonicators break particle agglomerates faster and much more thoroughly than bath-type sonicators. Since it is relatively quick, requires very little "high tech" equipment, and produces any number of nanofluids, this process is our method of choice. Unfortunately, surfactant-stabilized nanofluids are known to break down at elevated temperature [39]. For longer-term stability in a solar application, one can re-sonicate continuously or attempt more exotic preparation methods, such as those given in [34, 40].

To measure the optical properties, we used a spectrophotometer. This is a device that sends a light beam of variable wavelength through a sample and then detects the transmitted beam. Spectrophotometers come in several configurations and are good for a variety of wavelengths. For our purposes, we need measurements over the solar spectrum, i.e., between 0.20 to 3 μm. As such, we mostly use a Jasco V-670 (Jasco Corp., Great Dunmow, Essex, UK) which can take transmission measurements in the range of 0.19 to 2.7 μm, although other spectrophotometers are used for comparison in our testing.

*R*and transmission

*T*shown in Figure 4 in accordance with the approach of Large et al. [41]:

*n*

_{ i }and

*k*

_{ i }in the previous equations represent the

*i*th spectral real and imaginary components of the refractive index. Likewise,

*L*represents the length of the

*i*th element. To combine these equations for a two-element system, the following equations can be used [41]:

*k*

_{EXP}, a simple calculation can be performed to obtain the extinction coefficient,

*σ*

_{exp}. Equation 20 describes this final step [31]:

If our simplistic nanofluid model is accurate, *σ*_{EXP} should be directly comparable to the modeled quantity, *σ*_{total}, described in the previous section.

To determine the particle size in solution, dynamic light scattering (DLS) was done for selected materials - graphite (30 nm manufacturer-quoted average particle size (APS)) and silver (20 nm manufacturer APS). The equipment used to do these measurements was a Nicomp 380 DLS (Agilent Technologies, Inc., Santa Clara, CA, USA). Results gave volume-weighted average particle sizes to be 150 to 160 nm and 50 to 70 nm for graphite and silver, respectively. In both cases, the standard deviation was around half of the volume-weighted average. DLS testing also revealed that 24 h later the samples heavily clumped into 1 to 15 μm aggregates, showing that our preparation method for these fluids is only good for short-term stability. It should be noted that the volume-weighted average yields particle sizes that lie between number and intensity-weighted averages.

## Results and discussion

*k*

_{EXP}, to the extinction coefficients shown in the plot. For comparison, pure water with an excessive amount, 5% by volume, of surfactant is also shown. A high volume fraction surfactant was used to exaggerate the absorption of surfactant, which turns out to be very small.

The concentrations shown in Figure 5 represent a very wide range which could accommodate almost any solar receiver geometry. Overall, there is very good agreement between model and experimental results. Depending on volume fraction, the nanoparticles appear to be the absorbing material for shorter wavelengths (up to approximately 1 μm for 1 × 10^{-5} vol.% and up to approximately 2 μm for 0.1 vol.%), whereas at longer wavelengths, water becomes dominant and the curves converge. These results indicate that our simplistic approach (i.e., Equations 2 to 9) agrees well with experimental data.

Since the base fluid is a good absorber at longer wavelengths, it will also be a good emitter at those same wavelengths. That is, most nanofluids are also expected to have radiation losses nearing those of a blackbody at longer wavelengths (> 4 μm) according to Plank's radiation law. There are two possible solutions to this problem for a solar collector: (1) find a base fluid which has low emission for long wavelengths and (2) install a cover/glazing over the collector which will trap long-wavelength emitted radiation from leaving the system. The second solution is most likely to be adopted since (as mentioned above) there are many commercial materials which could be used to minimize losses and are still essentially transparent to the solar spectrum [26, 27].

Figure 6 also shows less agreement between the model results and the experimental results for metals than is seen for graphite. Most noticeably in silver, we expected to see a large peak in the extinction coefficient. This peak, referred to as the plasmon peak, is a built-in natural frequency where electrons will absorb and oscillate strongly in a metal. It is usually found in the range of 200 to 500 nm. However, our experimental results for metal-based nanofluid were rather constant and did not show a large, pronounced plasmon peak as expected. In general, our model for metal nanofluids appears to over-predict from very short wavelengths until around 600 to 700 nm where it then begins to under-predict the extinction coefficient.

The accuracy of this system is at least ± 0.3%*T*. Thus, if we get a result of 90% transmission, it could actually be 89.7% or 90.3% transmission. However, the poor match in results in Figures 6 and 7 cannot be explained by this error. One possible reason for the discrepancy, however, is that particle agglomerates are in the measurement beam path and absorb or scatter an anomalously large amount of light. That is, the real particle *shape* or *size* might deviate from the nominal manufacturer-stated nanoparticle specifications. Furthermore, the model assumes a monatomic particle distribution. That is, all the particles of a given sample are assumed to be the same size - thus, the average particle diameter quoted by the manufacturer. Another possible explanation for the poor agreement is that an oxide layer or other chemical deviation may occur in the metal nanoparticles giving different properties than that assumed in the bulk metal.

*σ*

_{total}and

*σ*

_{particles}are plotted together to demonstrate the effect of absorption by the base fluid. This shows the importance of adding in the extinction of the base fluid into the total result. Overall, Figure 8 shows that size effects, while very important, do not seem to explain the difference between the rather flat trend of the experimental results and the large peak in the theoretical model.

As mentioned above, scattering can also come into play, especially important at short wavelengths. Taking the results of Figure 8 and a nominal particle size of 100 nm, up to 5% of the incident light can be scattered in a solar nanofluid. In a 10-cm fluid depth, this translates to an average extinction coefficient of 0.05 cm^{-1}. Overall, these results show that a measurable amount of light can be scattered if large particles or particle agglomerates are present. If the particle size is < 50 nm, however, scattering is negligible - so care must be taken to make sure that the particles in a nanofluid stay "nano."

## Conclusions and future work

This article has shown measurement and modeling techniques for determining the optical properties of nanofluids. These two methods of determining optical properties are in very good agreement for graphite nanofluids. They also correspond well in the case of aluminum. However, experimental results did not match well with the model predictions for the other metals tested, particularly missing the large predicted plasmon peaks (e.g., silver). Particle size was discredited as the root of poor model predictions for metals. Scattering is expected to be negligible if care is taken to keep particles in solution near their manufacturer-listed diameters - so this is also unlikely to lead to significant errors. One possible explanation is purity of the materials. For instance, oxidization or other impurities on the particle surface might be responsible for the poor agreement with the model.

Solar thermal nanofluid comparison table

Type | Graphite | Al | Copper | Silver | Gold |
---|---|---|---|---|---|

Particle, vol.% | 0.0004 | 0.001 | 0.004 | 0.004 | 0.004 |

Commercially available | Yes | Yes | Yes | Yes | Yes |

Surfactant, vol.% | 0.5 | 0.25 | 0.25 | 0.25 | 0.25 |

1M NaOH, vol.% (achieve pH 9 to 10) | 0.003 | 0.003 | 0.003 | 0.003 | 0.003 |

Sonication time, min | 45 | 30 | 30 | 30 | 30 |

Collector depth, cm | 10 | 10 | 10 | 10 | 10 |

Approximate cost, $/L | 0.52 | 0.64 | 1.85 | 3.65 | 233 |

Further work will be necessary to obtain better models for nanofluids containing metallic nanoparticles other than aluminum. Also, a more in-depth study will be required to obtain optical properties at elevated temperatures. Since liquid-based solar thermal collectors can operate anywhere from 50°C to 500°C, it is very important to characterize these properties at those temperatures. We predict that nanofluids would be most cost-effectively placed into solar systems with a relatively small receiver area (such as a power tower or dish receiver), but more work must be done to determine the most advantageous use of solar nanofluids.

## Abbreviations

### NOMENCLATURE

*D*: Mean particle diameter (nm); *f*_{v}: Volume fraction (%); *I*: Irradiance, W m^{-2}; *k*: Complex component of the refractive index; L: Path length, mm; *m*: Relative complex refractive index (particles to fluid); *N*: Number of scatterers; *n*: Real component of the refractive index; *Q*: Optical efficiency factor; *R*: Reflectivity; *T*: Transmissivity.

#### Subscripts

║: Parallel component; ┴: Perpendicular component; abs: Absorption; e: Effective; ext: Extinction; EXP: Experimental result; F: Fluid; MOD: Modeling result; scat: Scattering.

#### Greek symbols

*α*: Particle size parameter; *ε'*: Real component of the dielectric constant, F/m or (kg mm mV^{-2} s^{-2}); *ε"*: Complex component of the dielectric constant, F/m or (kg mm mV^{-2} s^{-2}); *θ*: Scattering angle, radians; *λ*: Wavelength, μm; π: The constant, pi; *ρ*: Density, kg/m^{3} or #/m^{3}; *σ*: Extinction coefficient, 1/cm.

## Declarations

### Acknowledgements

The authors gratefully acknowledge the support of the National Science Foundation through award CBET-0932720.

## Authors’ Affiliations

## References

- Choi S, Siginer DA, Wang HP: Enhancing thermal conductivity of fluids with nanoparticles. Developments and applications of non-Newtonian flows.
*ASME*1995, 231(MD 66):99–105.Google Scholar - Prasher RS, Bhattacharya P, Phelan PE: Thermal conductivity of nanoscale colloidal solutions (nanofluids).
*Phys Rev Letters*2005, 94: 025901. 10.1103/PhysRevLett.94.025901View ArticleGoogle Scholar - Prasher RS, Phelan PE, Bhattacharya P: Effect of aggregation kinetics on the thermal conductivity of nanoscale colloidal solutions (nanofluids).
*Nano Letters*2006, 6: 1529–1534. 10.1021/nl060992sView ArticleGoogle Scholar - Taylor RA, Phelan PE, Otanicar T, Adrian RJ, Prasher RS: Vapor generation in a nanoparticle liquid suspension using a focused, continuous laser. Appl Phys Lett 95: 161907. 10.1063/1.3250174Google Scholar
- Otanicar T, Taylor RA, Phelan PE, Prasher R:
*Impact of size and scattering mode on the optimal solar absorbing nanofluid.*San Francisco: ASME ES; 2009:90066.Google Scholar - Bang IC, Chang SH: Boiling heat transfer performance and phenomena of Al
_{2}O_{3}**-water nano-fluids from a plain surface in a pool.***Int J Heat Mass Transfer*2005, 48(12):2420–2428. 10.1016/j.ijheatmasstransfer.2004.12.047View ArticleGoogle Scholar - Wang X-Q, Mujumdar AS: Heat transfer characteristics of nanofluids: a review.
*Int J Therm Sci*2007, 46: 1–19. 10.1016/j.ijthermalsci.2006.06.010View ArticleGoogle Scholar - Chopkar M, Das AK, Manna I, Das PK: Pool boiling heat transfer characteristics of ZrO
_{2}**-water nanofluids from a flat surface in a pool.***Heat Mass Transfer*2007, 44: 999–1004. 10.1007/s00231-007-0345-5View ArticleGoogle Scholar - Das SK, Putta N, Thiesen P, Roetzel W: Temperature dependence of thermal conductivity enhancement for nanofluids.
*ASME Trans J Heat Transfer*2003, 125: 567–574. 10.1115/1.1571080View ArticleGoogle Scholar - Eastman JA, Choi US, Li S, Thompson LJ, Lee S: Enhanced thermal conductivity through the development of nanofluids. In
*Proceedings of Materials Research Society Symposium, Boston, MA, USA*.*Volume 457*. Pittsburgh: Materials Research Society; 1997:3–11.Google Scholar - Gadhe JB, Gupta RB: Hydrogen production by methanol reforming in supercritical water: catalysis by in-situ-generated copper nanoparticles.
*Int J Hydrogen Energy*2007, 32: 2374–2381. 10.1016/j.ijhydene.2006.10.050View ArticleGoogle Scholar - Heris S, Etemad SG, Esfahany M: Experimental investigation of oxide nanofluids laminar flow convective heat transfer.
*Int Comm Heat Mass Transfer*2006, 33(4):529–535. 10.1016/j.icheatmasstransfer.2006.01.005View ArticleGoogle Scholar - Khanafer K, Vafai K, Lightstone M: Buoyancy-driven heat transfer enhancement in a two-dimensional enclosure utilizing nanofluids.
*Int J Heat Mass Transfer*2003, 46: 3639–3653. 10.1016/S0017-9310(03)00156-XView ArticleGoogle Scholar - Kim H, Kim J, Kim M: Experimental study on CHF characteristics of water-TiO2 nano-fluids.
*Nucl Eng Technol*2006, 38(1):61–68.Google Scholar - Kim SJ, Bang IC, Buongiorno J, Hu LW: Surface wettability change during pool boiling of nanofluids and its effect on critical heat flux.
*Int J Heat Mass Transfer*2007, 12: 4105–4116. 10.1016/j.ijheatmasstransfer.2007.02.002View ArticleGoogle Scholar - Klein JH, Karni J, Ben-Zvi R, Bertocchi R: Heat transfer in a directly irradiated solar receiver/reactor for solid-gas reactions.
*Solar Energy*2007, 81: 1227–1239. 10.1016/j.solener.2007.01.004View ArticleGoogle Scholar - Lapotko D, Lukianova E: Laser-induced micro-bubbles in cells.
*Int J Heat Mass Transfer*2005, 48: 227–234. 10.1016/j.ijheatmasstransfer.2004.08.012View ArticleGoogle Scholar - Merabia S, Keblinski P, Joly L, Lewis LJ, Barrat J-L: Critical heat flux around strongly heated nanoparticles.
*Physical Review E*2009, 79: 021404. 10.1103/PhysRevE.79.021404View ArticleGoogle Scholar - Truong BH: Determination of pool boiling critical heat flux enhancement in nanofluids. In
*Undergraduate thesis*. MIT; 2007.Google Scholar - You SM, Kim JH, Kim KH: Effect of nanoparticles on critical heat flux of water in pool boiling heat transfer.
*Appl Phys Lett*2003, 83: 3374–3376. 10.1063/1.1619206View ArticleGoogle Scholar - Tyagi H, Phelan PE, Prasher R: Predicted efficiency of a low-temperature nanofluid-based direct absorption solar collector.
*J Solar Energy Engineering*2009, 131(4):041004. 10.1115/1.3197562View ArticleGoogle Scholar - Otanicar TP, Phelan PE, Golden JS: Optical properties of liquids for direct absorption solar thermal energy systems.
*J Solar Energy*2009, 83: 969–977. 10.1016/j.solener.2008.12.009View ArticleGoogle Scholar - Otanicar T, Phelan PE, Prasher RS, Rosengarten G, Taylor RA: Nanofluid-based direct absorption solar collector.
*J Renewable and Sustainable Energy*2010, 2: 033102. 10.1063/1.3429737View ArticleGoogle Scholar - Lenert A, Zuniga YSP, Wang EN:
*Nanofluid-based absorbers for high temperature direct solar collectors.*Washington, DC; 2010:22208. IHTC14Google Scholar - Banerjee D, Shin D: Enhanced specific heat capacity of molten salt-metal oxide nanofluid as hear transfer fluid for solar thermal applications.
*SAE International*2010. Paper No. 2010–01–1734 Paper No. 2010-01-1734Google Scholar - Edmund Optics, Anti-Reflection (AR) Coated High Efficiency Windows2011. [http://www.edmundoptics.com/onlinecatalog/displayproduct.cfm?productID=1919] Accessed Jan
- Schott, Specialty Glasses and Materials2011. [http://www.us.schott.com/advanced_optics/english/our_products/materials/specialty_glass/index.html] Accessed Jan
- Prasher R, Song D, Wang J, Phelan P: Measurements of nanofluid viscosity and its implications for thermal applications.
*Appl Phys Lett*2006, 89: 133108. 10.1063/1.2356113View ArticleGoogle Scholar - Palik E:
*Handbook of optical constants of solids.*London: Elsevier; 1998.Google Scholar - Tien CL: Thermal radiation in packed and fluidized beds.
*J Heat Transfer*1988, 110: 1230–1242. 10.1115/1.3250623View ArticleGoogle Scholar - Modest MF:
*Radiative heat transfer.*2nd edition. Massachusetts: Academic; 2003.Google Scholar - Bohren CF, Huffman DR:
*Absorption and scattering of light by small particles.*New York: Wiley; 1998:287–324.View ArticleGoogle Scholar - Lo CH, Tsung TT, Chen LC: Shaped-controlled synthesis of Cu-based nanofluid using submerged arc nanoparticle synthesis system (SANSS).
*J Cryst Growth*2005, 277(1):636–642. 10.1016/j.jcrysgro.2005.01.067View ArticleGoogle Scholar - Bromberg L, Raduyk S, Hatton TA: Functional magnetic nanoparticles for biodefense and biological threat monitoring and surveillance.
*Analytical Chemistry*2009, 81: 5637–5645. 10.1021/ac9003437View ArticleGoogle Scholar - Wei X, Zhu H, Kong T, Wang T: Synthesis and thermal conductivity of Cu
_{2}O nanofluids.*Int J Heat Mass Transfer*2009, 52: 4371–4374. 10.1016/j.ijheatmasstransfer.2009.03.073View ArticleGoogle Scholar - Advanced Materials 'Nanopowders'[http://www.advancedmaterials.us/nanomat.htm]
- Sigma-Aldrich 'Nanopowders'[http://www.sigmaaldrich.com/materials-science/nanomaterials/nanopowders.html]
- NanoAmor, 'Catalog of Nanoscale Particulate Materials' NanoStructured and Amorphous Materials, Inc[http://www.nanoamor.com/cat/catalog_nanoamor.pdf]
- Wen D, Ding Y: Experimental investigation into the pool boiling heat transfer of aqueous based γ-alumina nanofluids.
*J Nanopart Res*2005, 7: 265–274. 10.1007/s11051-005-3478-9View ArticleGoogle Scholar - Hwang Y, Lee JK, Lee CH, Jung Y, Cheong SI, Lee CG, Ku BC, Jang SP: Stability and thermal conductivity characteristics of nanofluids.
*Thermochimica Acta*2007, 455: 70–74. 10.1016/j.tca.2006.11.036View ArticleGoogle Scholar - Large MCJ, McKenzie DR, Large MI: Incoherent reflection process: a discrete approach.
*Optics Communications*1996, 128: 307–314. 10.1016/0030-4018(95)00761-XView ArticleGoogle Scholar

## Copyright

This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.

## Comments

View archived comments (2)